# Question 7.1: Design of a Nondestructive Test A large steel plate used in ......

Design of a Nondestructive Test
A large steel plate used in a nuclear reactor has a plane strain fracture toughness of 80,000 psi $\sqrt{in.}$ and is exposed to a stress of 45,000 psi during service. Design a testing or inspection procedure capable of detecting a crack at the edge of the plate before the crack is likely to grow at a catastrophic rate.

Step-by-Step
The 'Blue Check Mark' means that this solution was answered by an expert.

We need to determine the minimum size of a crack that will propagate in the steel under these conditions. From Equation 7-1 assuming that f = 1.12 for a single-edge notch crack:

$K=f \sigma \sqrt{\pi a}$     (7-1)
$K_{Ic}=f \sigma \sqrt{\pi a}$
$80,000 \ psi \ \sqrt{in.}=(1.12)(45,000 \ psi) \sqrt{\pi a}$
$a= 0.8 \ in.$

A 0.8 in. deep crack on the edge should be relatively easy to detect. Often, cracks of this size can be observed visually. A variety of other tests, such as dye penetrant inspection, magnetic particle inspection, and eddy current inspection, also detect cracks much smaller than this. If the growth rate of a crack is slow and inspection is performed on a regular basis, a crack should be discovered long before reaching this critical size.

Question: 7.7

## Strength of Ceramics and Probability of Failure An advanced engineered ceramic has a Weibull modulus m = 9. The flexural strength is 250 MPa at a probability of failure F = 0.4. What is the level of flexural strength if the probability of failure has to be 0.1? ...

We assume all samples tested had the same volume; ...
Question: 7.13

## Design of Links for a Chain Design a ductile cast iron chain (Figure 7-27) to operate in a furnace used to fire ceramic bricks. The chain will be used for five years at 600°C with an applied load of 5000 lbs. ...

From Figure 7-26(b), the Larson-Miller parameter f...
Question: 7.12

## Failure Analysis of a Pipe A titanium pipe used to transport a corrosive material at 400°C is found to fail after several months. How would you determine the cause for the failure? ...

Since a period of time at a high temperature was r...
Question: 7.11

## Design of a Fatigue Resistant Plate A high-strength steel plate (Figure 7-20), which has a plane strain fracture toughness of 80 MPa√m is alternately loaded in tension to 500 MPa and in compression to 60 MPa. The plate is to survive for ten years with the stress being applied at a frequency of once ...

To design our manufacturing and testing capability...
Question: 7.10

## Design of a Rotating Shaft A solid shaft for a cement kiln produced from the tool steel in Figure 7-18 must be 96 in. long and must survive continuous operation for one year with an applied load of 12,500 lb. The shaft makes one revolution per minute during operation. Design a shaft that will ...

The fatigue life required for our design is the to...
Question: 7.9

## Fatigue Failure Analysis of a Crankshaft A crankshaft in a diesel engine fails. Examination of the crankshaft reveals no plastic deformation. The fracture surface is smooth. In addition, several other cracks appear at other locations in the crankshaft. What type of failure mechanism occurred? ...

Since the crankshaft is a rotating part, the surfa...
Question: 7.8

## Weibull Modulus Parameter Determination Seven silicon carbide specimens were tested and the following fracture strengths were obtained: 23, 49, 34, 30, 55, 43, and 40 MPa. Estimate the Weibull modulus for the data by fitting the data to Equation 7-11. Discuss the reliability of the ceramic. ...

First, we point out that for any type of statistic...
Question: 7.6

## Fracture in Composites Describe the difference in fracture mechanism between a boron-reinforced aluminum composite and a glass fiber-reinforced epoxy composite. ...

In the boron-aluminum composite, the aluminum matr...
Question: 7.5